## Indium Thin Films in

## Multilayer Superconducting

## Quantum Circuits

by

### Corey Rae Harrington McRae

A thesis

presented to the University of Waterloo in fulfillment of the

thesis requirement for the degree of Doctor of Philosophy

in

Physics (Quantum Information)

Waterloo, Ontario, Canada, 2018

Examining Committee Membership

The following served on the Examining Committee for this thesis. The decision of the Examining Committee is by majority vote.

External Examiner Robert McDermott

Professor

Supervisor Matteo Mariantoni

Assistant Professor

Co-Supervisor Raymond Laflamme

Professor

Internal Member Robert Hill

Associate Professor Internal-External Member Guo-Xing Miao

Assistant Professor

Internal Member Crystal Senko

This thesis consists of material all of which I authored or co-authored: see Statement of Contributions included in the thesis. This is a true copy of the thesis, including any required final revisions, as accepted by my examiners.

Statement of Contributions

The content of Chapter 3was published on 2017 September 18 as [1] :

McRae, C.R.H., B´ejanin, J.H., Pagel, Z., Abdallah, A.O., McConkey, T.G., Earnest, C.T., Rinehart, J.R., Mariantoni, M. Thermocompression Bonding Technology for Multi-layer Superconducting Quantum Circuits. Appl. Phys. Lett. 111, 123501 (2017).

Author Contributions

Matteo Mariantoni, Thomas McConkey, and Corey Rae McRae conceived of the study. Corey Rae McRae designed the devices for this project.

Thomas McConkey and Corey Rae McRae performed device simulations. Corey Rae McRae developed the device fabrication processes.

Carolyn Earnest and Corey Rae McRae fabricated the devices.

Adel Abdallah, Matteo Mariantoni, Corey Rae McRae, and Zachary Pagel performed bonding development, set-up, and execution.

J´er´emy B´ejanin, Matteo Mariantoni, Thomas McConkey, and John Rinehart performed measurement set-up and calibration.

J´er´emy B´ejanin, Matteo Mariantoni, and Corey Rae McRae performed device cooldowns and measurements.

Matteo Mariantoni and Corey Rae McRae wrote the first draft of the manuscript. All authors contributed to the final version.

The content of Chapter4 was submitted on 2017 December 22 as:

McRae, C.R.H., B´ejanin, J.H., Earnest, C.T., McConkey, T.G., Rinehart, J.R., Deimert, C., Thomas, J., Wasilewski, Z.R., Mariantoni, M. Thin Film Metrology and Microwave Loss Characterization of Indium and Aluminum/Indium Superconducting Planar Resonators. J. Appl. Phys. (2017).

Author Contributions

Matteo Mariantoni and Corey Rae McRae conceived of the study. Corey Rae McRae designed the devices for this project.

Joseph Thomas, Chris Deimert, and Zbig Wasilewski performed molecular beam epi-taxy depositions and some materials characterization.

Carolyn Earnest and Corey Rae McRae fabricated the devices.

J´er´emy B´ejanin, Thomas McConkey, John Rinehart, and Matteo Mariantoni performed measurement set-up and calibration.

J´er´emy B´ejanin, Carolyn, Earnest, Thomas McConkey, Corey Rae McRae, and Matteo Mariantoni performed the device cooldowns and measurements.

Abstract

The superconducting quantum computer is an implementation of the quantum com-puter and a current leader the field in terms of performance and potential for scalability to large systems. Its two main components are the superconducting microwave resonator and the quantum bit (qubit). In Chapter 1, the concept of quantum computing is introduced, and the superconducting microwave resonator is explained in depth, along with a glimpse at the qubit and a description of two level system loss, the most prominent form of loss in low-power superconducting quantum circuits.

Scalability is essential to the development of fault-tolerant quantum computing, as error correction requires a large array of quantum bits. The multilayer quantum circuit archi-tecture is rising to the forefront as a solution to many of the scalability issues facing the field today. Chapter 2summarizes some of these scalability issues, such as the suppression of unwanted modes and materials losses, and presents an overview of multilayer architec-tures applied to superconducting quantum circuits. The chapter further delves into indium bump bonding, an essential technique in multilayer circuit fabrication.

In Chapter3, we experimentally demonstrate a thermocompression bonding technology between on-chip indium thin films and apply it to capped superconducting devices. These devices can be used as a building block towards a more scalable architecture: the multilayer quantum circuit. We characterize the dc and microwave performance of these bonded devices at room temperature as well as cryogenic temperatures. At 10 mK, we find a small but significant dc bond resistance of 49.2µΩ cm2. A tunnel-capped, bonded device shows minimal microwave reflections and clean transmission up to 6.8 GHz compared to a similar uncapped device, demonstrating good performance. As a proof of concept, we fabricate and measure a set of tunnel-capped superconducting resonators, demonstrating marginal deterioration in resonator performance due to the bonding procedure. This work demonstrates that thermocompression bonding between thin on-chip indium films is a useful addition to the multilayer quantum circuit toolbox, and that this technique, when applied to form the tunnel-capped superconducting device, shows a promising step towards more scalable architectures.

Indium is becoming ubiquitous in superconducting microwave circuits as it continues to be widely adopted as a bonding medium. However, the loss mechanisms in superconducting indium films have not been examined until now. In Chapter4, we characterize microwave loss in indium and aluminium/indium thin films on silicon substrates by measuring su-perconducting coplanar waveguide resonators and estimating the main loss parameters at powers down to the sub-photon regime and at temperatures between 10 and 450 mK. We

compare films deposited by thermal evaporation, sputtering, and molecular beam epitaxy. We study the effects of heating in vacuum and ambient atmospheric pressure as well as the effects of pre-deposition wafer cleaning using hydrofluoric acid. The microwave measure-ments are supported by thin film metrology including secondary-ion mass spectrometry. For thermally evaporated and sputtered films, we find that two-level states (TLSs) are the dominating loss mechanism at low photon number and temperature. Thermally evaporated indium is determined to have a TLS loss tangent due to indium oxide of ∼ 5 × 10−5. The molecular beam epitaxial films show evidence of formation of a substantial indium-silicon eutectic layer, which leads to a drastic degradation in resonator performance.

Acknowledgements

Thanks to the members of my committee: Matteo Mariantoni, Raymond Laflamme, Robert Hill, Guo-Xing Miao, Crystal Senko, and especially Robert McDermott.

Thanks go out to my fellow members of the Laboratory for Digital Quantum Matter. I couldn’t have done it without the long hours of fab troubleshooting with Cary, the long hours of measurement troubleshooting with J´er´emy, and the long hours of simulation troubleshooting with Thomas.

I am grateful for the guidance and expertise of the staff at the University of Waterloo’s Quantum Nanofab facility, especially Nathan, Brian, and Vito.

I could not have completed my degree without the love, support, and patience of my family: Mike, Marni, Ken, and Molly, and my other family: Alice, Gertrude, and Gina.

Dedication

## Table of Contents

List of Tables xiv

List of Figures xvi

1 Introduction 1

1.1 The resonator . . . 3

1.1.1 The lumped element circuit . . . 3

1.1.2 The distributed element circuit . . . 7

1.1.3 Modes . . . 10

1.1.4 Resonator quantization . . . 10

1.1.5 The coplanar waveguide . . . 12

1.2 The qubit . . . 16

1.3 Two level system loss . . . 17

1.3.1 The two level system Hamiltonian . . . 18

1.3.2 Dielectric contribution of TLSs . . . 19

2 Moving towards extensibility and scalability 21 2.1 Understanding and suppressing unwanted modes and coupling . . . 22

2.1.1 Slotline modes. . . 22

2.1.2 Crosstalk . . . 23

2.1.4 Identifying unwanted coupling . . . 27

2.2 Multilayer quantum devices . . . 27

2.2.1 Indium in multilayer quantum circuits . . . 29

3 Indium thin film thermocompression bonding for multilayer supercon-ducting quantum circuits 32 3.1 Introduction . . . 33

3.2 Sample fabrication . . . 35

3.3 Thermocompression bonding . . . 36

3.3.1 Bonding details . . . 36

3.3.2 Bonding recipe . . . 38

3.3.3 Bonding results and next steps . . . 39

3.4 Dc characterization of capped devices . . . 40

3.4.1 Measurement set-up and settings . . . 42

3.5 Bond inhomogeneity . . . 45

3.5.1 Interdiffusion and bonding . . . 45

3.5.2 Visual characterization of bond area . . . 45

3.5.3 Scanning acoustic microscopy characterization . . . 46

3.5.4 The flux tube model . . . 47

3.5.5 Bond superconductivity . . . 49

3.5.6 Indium film transition temperature . . . 49

3.6 Microwave characterization of capped devices . . . 50

3.6.1 Reflection measurements . . . 50

3.6.2 Reflection simulations of the tunnel mouth . . . 51

3.6.3 Crosstalk measurements . . . 51

3.6.4 Transmission measurements . . . 53

3.7.2 Capped and uncapped resonator comparison . . . 55

3.7.3 Vacuum contribution to capped resonators quality factor . . . 55

3.8 Conclusions and outlook . . . 58

4 Thin film metrology and microwave loss characterization of indium and aluminum/indium superconducting resonators 60 4.1 Introduction . . . 61

4.2 Loss mechanisms and motivation . . . 62

4.3 Film deposition and fabrication . . . 63

4.4 Thin film metrology. . . 67

4.4.1 Surface morphology and crystallinity . . . 68

4.4.2 Silicon/indium interdiffusion . . . 69

4.4.3 Si/Al/In interdiffusion . . . 70

4.4.4 Surface oxides . . . 70

4.5 Circuit layout and transmission-coefficient measurements . . . 73

4.6 Resonator measurements . . . 75

4.6.1 Photon number sweeps . . . 75

4.6.2 Temperature sweeps of thermally evaporated In resonators . . . 76

4.6.3 Temperature sweeps of sputtered Al/In resonators . . . 77

4.7 Results and discussion . . . 77

4.8 Conclusion . . . 79

5 Conclusion 81 5.1 Indium thin film thermocompression bonding for multilayer superconducting quantum circuits . . . 81

5.2 Thin film metrology and microwave loss characterization of indium and alu-minum/indium superconducting resonators . . . 82

APPENDICES 90

A Nanofabrication and microfabrication 91

A.1 Mask design tips . . . 91

A.1.1 Alignment marker design . . . 92

A.1.2 Wafer and die manipulation . . . 93

A.1.3 Compatibility with measurement set-up. . . 93

A.2 Silicon wafers . . . 94

A.2.1 Intrinsic silicon . . . 95

A.2.2 Silicon ingot growth methods . . . 95

A.3 Appropriate glassware . . . 95

A.4 Aluminium/indium superconducting quantum circuit process . . . 96

A.5 Indium superconducting quantum circuit process . . . 97

A.6 Aluminium/indium cap process . . . 97

A.7 Aluminium superconducting quantum circuits process . . . 99

A.8 RCA silicon wafer surface cleaning . . . 101

A.8.1 RCA SC-1 process . . . 103

A.8.2 HF dip process . . . 104

## List of Tables

3.1 Aluminium and indium film deposition parameters. . . 36

3.2 Type and quantity of all bonded samples.. . . 39

3.3 Samples and relative SMU settings for all reported dc measurements. . . . 43

3.4 Resonator parameters. . . 57

4.1 Description of In and Al/In films characterized in this experiment. “De-position and metal(s):” Type of de“De-position and metal or metals deposited onto sample, in order of deposition. “Other processing:” Extra steps per-formed on sample either before or after deposition. “Design:” CPW trans-mission line design type 1 or 2. “t1; t2:” Deposited film thickness for Al and In, respectively. “TE:” Thermally evaporated film (i.e., unprocessed film). “Heated:” Post-patterning heating in ambient atmospheric pressure. “HF:” Pre-deposition cleaning with RCA SC-1 and HF dip. “S:” Sputtered film (i.e., unprocessed film). “Heated Vacuum:” Post-patterning heating in vac-uum. “MBE:” Molecular beam epitaxial film. “Annealed:” Post-deposition annealing in UHV. Thermally evaporated and sputtered films are deposited on high-resistivity (> 10 kΩ cm) 500µm thick 3-in. float-zone (FZ) undoped Si (100) wafers; MBE films are deposited on 3-in. Si (001) wafers. . . 64

4.2 Surface oxide analysis for all unheated samples and non-annealed MBE sam-ple described in Table 4.1. “Samsam-ple:” Samsam-ple type (see Table 4.1). “tInO:” Native In oxide thicknesses; “tSiO:” Native Si oxide thicknesses. Two dif-ferent spots [(A) and (B)] on the Si (gap) surface for the sputtered Al/In sample are measured. . . 71

4.3 Quantitative analysis of loss mechanisms for the three thermally evaporated In samples. “1/Qi(hnphi):” S-curve measurements used to estimate F tan δTLS and 1/QHP. “1/Qi(T ) Fit:” Temperature sweep measurements used to esti-mate F tan δ0

TLSand 1/Q∗ as fitting parameters. “∆ ˜f (T ) Fit:” Temperature
sweep measurements used to estimate F tan δ0_{TLS} and f_{0}0 as fitting
parame-ters. Each fitting parameter is reported with its standard deviation. . . 80

## List of Figures

1.1 Lumped element RLC circuit. . . 4

1.2 Complex Lorentzian function. . . 6

1.3 Distributed element circuit. . . 8

1.4 Diagram of standard CPW and GCPW. . . 15

1.5 Potential energy diagram for a double well potential. . . 18

2.1 Physical implementations of two common solutions to parasitic slotline modes. 24 2.2 Image of a microwave package containing a set of six three-dimensional wires. 25 2.3 Cross-sectional diagram of a shielded coplanar transmission line designed to suppress unwanted modes and crosstalk. . . 26

2.4 Cross-sectional diagram of a sample box with under-chip cavity. . . 27

2.5 Simulation of the first box mode in a large sample box with 89 coaxial pogo pins. . . 28

2.6 The microwave multilayer integrated quantum circuit. . . 30

3.1 Capped devices formed using thermocompression bonding in vacuum. . . . 34

3.2 Thermocompression bonding setup. . . 37

3.3 Bond characterization at dc. . . 41

3.4 SMU characterization at dc with a superconducting aluminium sample. . . 44

3.5 Optical characterization of bond inhomogeneity. . . 46

3.6 Scanning acoustic microscopy image of capped test sample. . . 47

3.8 Resistance R as a function of temperature T for a capped device. . . 50

3.9 Tunnel mouth simulations. . . 52

3.10 Characterization at microwave frequencies of the uncapped and capped CPW transmission lines. . . 54

3.11 Uncapped and capped resonator measurements at low power. . . 56

4.1 RHEED images. (a) Si wafer during oxide desorption at 1010◦C (after pre-cleaning). (b) Si wafer after oxide desorption and after cooling to ∼ 0◦C. (c) and (d) Immediately post-growth images for the MBE In and MBE In annealed films, respectively. The film in (d) shows a polycrystalline pattern during growth, with the shown image being captured after additional annealing. The hazy background may indicate the presence of a disordered phase in addition to the single-crystal phase. . . 65

4.2 DIC microscopy (background) and standard optical microscopy (insets) of In and Al/In sample surfaces, showing surface and device edge roughness, respectively. Standard microscope images show a CPW transmission line running top to bottom with gaps exposing the Si substrate. Samples shown are thermally evaporated In in (a), thermally evaporated In heated in (b), thermally evaporated In HF in (c), sputtered Al/In in (d), MBE In in (e), and MBE In annealed in (f). Sample details are reported in Table 4.1.. . . 66

4.3 Characterization of In/Si interdiffusion. SEM image of a cleaved thermally evaporated In HF sample (a) and MBE In sample (b). D-SIMS depth profil-ing for the thermally evaporated In HF sample (c) and MBE In sample (d) showing measured intensity in counts per second (cps), I, vs. depth, d. Solid lines: Si counts; dashed lines: In counts. Layer i: 1µm deep In layer; layer ii: Top part of Si substrate. Layer separation indicated by vertical dotted black lines. The insets show the D-SIMS crater profile plotted as depth d vs. crater diameter, `. . . 68

4.4 Photon number sweeps (S-curves). Intrinsic quality factor Qi vs. mean pho-ton number hnphi for samples described in Table 4.1. The horizontal dashed black lines indicate the estimated values of the high photon number quality factor QHP and low photon number quality factor QLP for the thermally evaporated In sample. The measurement setup and estimation of hnphi are the same as in [27]. . . 71

4.5 Characterization of Si/Al/In interdiffusion. D-SIMS depth profiling for the sputtered Al/In sample [dark blue (dark gray)] and sputtered Al/In heated sample [light blue (light gray)] showing measured intensity in counts per second (cps), I, vs. depth, d. Dashed lines: In counts; dotted lines: Al counts; solid lines: Si counts. Layer i: 150 nm deep In layer; layer ii: 150 nm deep Al layer; layer iii: Top part of Si substrate. Layer separation indicated by vertical dotted black lines. . . 72

4.6 Transmission-coefficient measurements. Magnitude of the measured trans-mission coefficient kS21k vs. f . Inset: Circuit layout of design 1 (left) and design 2 (right). In both layouts, the measured CPW transmission lines are those between ports 1 and 2. . . 74

4.7 Temperature sweeps. Loss tangent 1/Qi(a) and normalized frequency shift ∆ ˜f (b) vs. hf0/(kBT ) for the three thermally evaporated In samples presented in Table 4.1. The resonance frequencies at T = 10 mK used in the x-axes are reported in Subsec. 4.6.1. TLS model fitting curves obtained from Eqs. (4.3) and (4.4) (solid lines) with standard deviation bands (shaded areas) are over-laid to data points for unprocessed (open circles), heated (open triangles), and HF (open squares) samples. . . 77

4.8 Temperature sweeps. 1/Qi (a) and ∆ ˜f (b) vs. hf0/(kBT ) for the two sputtered Al/In samples presented in Table 4.1. TLS model fitting curves (dashed lines) are overlaid to data points for unprocessed (open diamonds) and heated (stars) samples. . . 78

## Chapter 1

## Introduction

The classical computer has altered the way humans live in almost every aspect, from medical breakthroughs to social media to agriculture and manufacturing. Many of the contexts in which classical computers are used today were inconceivable to people living in the pre-digital world. It would have been impossible to predict all of the ways in which computers would become embedded into the world around us. Similarly, it is difficult to envision a world in which quantum computers1 are ubiquitous. Currently, quantum computing is changing the way we face cryptography [2] and shows promise as a simulation tool in molecular chemistry [3] and machine learning [4]. If history is any indication, the full impact of the field of quantum computing will not be uncovered until long after the quantum computer becomes a reality.

The quantum computer is composed of a set of qubits. Each qubit can be in state |0i,
state |1i, or a linear combination of these two states, α |0i+β |1i where α and β are complex
values. Qubits can be initialized to the |0i or |1i state, can interact with themselves and
one another through quantum gates, and can be measured, giving a classical output of 0
or 1. A measurement of the state α |0i + β |1i will give 0 with probability |α|2 and 1 with
probability |β|2_{.}

A variety of quantum computer implementations are currently being considered and researched in depth. Types of physical realizations include [5] :

• Trapped atoms, where qubits consisting of isolated ions are manipulated using lasers; • Quantum dots, where qubits consist of a single electron or hole isolated by impurities

• Nuclear magnetic resonance (NMR), where qubits are defined as the nuclear spin of elements in a large molecule and subjected to a magnetic field, and gates are performed using radio-frequency (RF) pulses;

• Optical quantum computing, where individual photons act as qubits and manipula-tion is performed on an optical table;

• And superconducting quantum computing, where qubits are composed of a combi-nation of LC circuits and nonlinear quantum oscillators called Josephson junctions and are controlled by microwave pulses.

In this thesis, we delve into the superconducting quantum computing realization of the quantum computer. This area is a leader in the field of quantum computing with high qubit coherence times, good control and measurement, and the promise of an imple-mentable quantum error correction algorithm, the surface code [6, 7]. Architectures based on superconducting qubits are improving rapidly, and are approaching the realm of higher performance over the leading classical supercomputer [8].

In practice, the superconducting quantum circuit is a set of on-chip devices that are controlled using low power RF pulses and operated at temperatures near 10 mK. These circuits are made up of three major components: the transmission line, the resonator, and the qubit.

Qubits are the source of the quantum information, and are connected to input and output electronics through transmission lines and resonators. The experiments in this work are performed using superconducting quantum circuits with transmission lines and resonators only. Transmission lines act as a wire to propagate the microwave signal from one location to another, while resonators hold a signal of a specific frequency depending on their length and can couple to other devices to pass this signal along.

Resonators are a convenient tool to measure the performance of a circuit due to its material make-up or the processing it has undergone. The performance of an individual resonator is measured by its internal quality factor, Qi. Qi can be determined by fitting

to the transmission of the resonator as a function of microwave frequency. By performing these fits at a variety of temperatures and powers, information can be determined about loss mechanisms within the circuit.

The upcoming sections in this chapter will introduce the resonator and the qubit as elements in the superconducting quantum circuit, and explain the concept of the nebulous two-level system and its effect on superconducting circuit performance.

### 1.1

### The resonator

Superconducting microwave resonators are an essential part of the superconducting quan-tum circuit architecture. They are used as buses between qubits, short-term storage, and circuit control and readout. The most common type of resonator in superconduct-ing circuits is the coplanar waveguide (CPW) resonator, which consists of a ssuperconduct-ingle surface supporting a centre conductor with ground planes on either side and dielectric below (see Sec. 1.1.5 for more details on the CPW).

Resonators can be designed in a lumped element circuit model (consisting of discrete capacitive, inductive and resistive components) or a distributed element model (consisting of a length of circuit with a capacitance, inductance and resistance per unit length) [9,10]. We begin by examining the simpler lumped element model and use it to develop an intuition for the quality factor. Then we move to the distributed element model, which characterizes the CPW. We briefly introduce the concept of modes, as well as the quantization of the resonator circuit model. Finally, we explore CPW behaviour in detail [11].

### 1.1.1

### The lumped element circuit

Many concepts crucial to the superconducting CPW resonator are shared with the lumped element circuit. Thus, we can build an intuition for the superconducting microwave res-onator by exploring the behaviour of the lumped element circuit. In this section, two critical variables used to characterize a resonator are introduced: the resonant frequency and the quality factor. The Lorentzian behaviour of the resonator is also examined. This section is based on the treatment of the lumped element resonant circuit in Collin [9] and Mariantoni [10].

A circuit with resistive, inductive, and capacitive elements (an RLC circuit) can have connections in series or in parallel. The input impedance of a series RLC circuit (Fig.1.1(a)) is

Zin = R + j(ωL −

1

ωC) (1.1)

where R is the resistance, L is the inductance, C is the capacitance, ω is the angular frequency, and j =√−1.

Zinis exclusively real when the frequency is such that the imaginary component is zero,

i.e.

ω0 =

1

(a) C (b) L R I V C L 1/R I V

Figure 1.1: A series (a) and parallel (b) lumped element RLC circuit with capacitance C, inductance L, resistance R, voltage V and input current I.

This is the resonant frequency of the circuit. We can determine the time-averaged energies stored in the electric and magnetic field (i.e. in the capacitor and inductor) as

WC =
1
4CV
∗
CVC (1.3)
WL=
1
4LI
∗_{I} _{(1.4)}

where I is the input current and VC is the voltage across the capacitor. The total

time-averaged energy of the system is W = WC + WL. By rewriting the input impedance in

terms of W_{C} and W_{L}, it becomes evident that to achieve a real input impedance and
circuit resonance, we must have WC = WL. Thus, at resonance, the time-averaged energy

is shared equally between the capacitor and the inductor.

When considering resonant circuits, the quality factor Q becomes an important concept.
Q indicates circuit performance and takes into account loss within the circuit. Broadly, we
define
Q = 2πωW
PR
(1.5)
where
PR=
1
2RI
∗_{I} _{(1.6)}

is the power loss due to the resistor. Thus, in general terms, the quality factor describes the energy loss ratio of the system.

The quality factor for a series RLC resonator reduces to Qs = 2π

ωRC = 2πωL

by substituting the average energy W = WC + WL= 2WC = 2WL= 1_{2}LI∗I.

For frequencies close to resonance, ω = ω0 + ∆ω we can approximate 1/ω ' (1 −

∆ω/ω0)/ω0 which, when substituted, gives

Zin = R + j(ω0+ ∆ω)L − j

1 − ∆ω/ω0

ω0C

. (1.8)

In terms of the quality factor and relative frequency shift, we can say Zin = 1 R 1 + j2Q s 2π ∆ω ω0 . (1.9)

The inverse of the input impedance is called the input admittance, Y_{in} = Z_{in}−1. For a
series RLC circuit, Yin is a complex Lorentzian function that illustrates typical resonance

behaviour. The magnitude of Yin is

|Yin| =
1
Rq1 + 4(Q_{2π}s)2_{(}∆ω
ω0)
2
(1.10)

and its phase is

∠Yin= arctan −2Q s 2π ∆ω ω0 . (1.11)

∠Yin and the normalized version of the magnitude, |Yin|/Gs, where Gs = 1/R is the

conductance, are plotted in Fig. 1.2. We expect a similar response from superconducting microwave resonator measurements, as explained in Sec.1.1.2.

By rearranging (1.9) and substituting Qs/2π = 1/Rω0C, we can obtain

Zin = R + j2L∆ω. (1.12)

We can also define the quality factor in terms of its 3 dB bandwidth, κ = ω2− ω1, where

ω1 and ω2 are frequencies at which |Yin|/Gs is 3 dB lower than its peak value. Then:

Qs = ω0

κ . (1.13)

A similar derivation to the above can be shown for parallel RLC circuits. In contrast to (1.9),

Zin =

R

−4 −2 0 2 4
0
0.2
0.4
0.6
0.8
1
|Y
in
|/
G
s
−4 −2 0 2 4
−2
−1
0
1
2
∆ω/ω0
∠
Yin
Qs _{= 5}
Qs _{= 10}
Qs _{= 15}
(a)
(b)

Figure 1.2: Normalized magnitude |Yin|/Gs (a), and phase ∠Yin (b), of the complex

Lorentzian function laid out in (1.10) and (1.11) for increasing values of the quality factor Qs. The magnitude of the Lorentzian curve peaks at the resonant frequency ω0. This peak

for a parallel RLC circuit.

The quality factor can be broken down into components based on the source of loss
that is represented in R. The internal quality factor, Q_{i}, is composed of loss within the
circuit. This is the value we have been referring to in this chapter when using the general
term quality factor. The coupled quality factor, Qc, is added to the mix when the circuit

is influenced by the presence of an external load resistor in series, which can represent coupling of the device to other systems such as an on-chip transmission line. The loaded quality factor, Ql, takes into account both of these sources of loss, as:

1 Ql = 1 Qc + 1 Qi . (1.15)

### 1.1.2

### The distributed element circuit

The distributed element circuit is defined by values of resistance, inductance and capaci-tance which are spread throughout the circuit rather than located at discrete points within it. In this section, we lay out the distributed element circuit model and explore the effect of various line terminations. We demonstrate how a shorted and an open distributed ele-ment circuit can be approximated to a series RLC lumped eleele-ment circuit, confirming the validity of the simpler lumped model applied to a CPW. This introduction to distributed element circuits is based on information found in Collin [9] and Mariantoni [10].

To accurately study the transmission line, we must take into account that its capaci-tance, inductance and resistance is not concentrated at a single point but rather distributed over a length of material. Distributed element devices tend to be less lossy than their lumped counterparts, and are therefore more commonly used in superconducting quantum circuits [10].

A transmission line of length z = ` can be modeled as two wires, one conductor and one ground, separated by a length of dielectric and terminated at each end by load resistance ZL (Fig. 1.3). For infinitesimal segment dz, the conductor has input current I(z), output

current I(z+dz), and series inductance and resistance ldz and rdz. It also has a capacitance to ground cdz, parallel conductance gdz, and input and output voltages V (z) and V (z+dz). The line’s characteristic impedance

Z0 = p l/c, (1.16) attenuation constant α = 1 r 1 + gZ (1.17)

... ... r dz l dz g dz c dz I(z) V(z) I(z+dz) V(z+dz)

Figure 1.3: Distributed element circuit showing an expanded version of infinitesimal seg-ment dz. Each segseg-ment has input current I(z), output current I(z + dz), series inductance ldz, series resistance rdz, capacitance to ground cdz, parallel conductance gdz, and input and output voltages V (z) and V (z + dz).

and propagation phase constant

β = ω c0

≈ ω√lc (1.18)

are used to characterize the properties of the line. Note that we assume nondispersivity2 and low loss through the line.

For now we will assume negligible dielectric losses since dielectric materials common in superconducting quantum circuits are low loss.3 In that case, g = 0 and

α = r/2Z0. (1.19)

The input impedance of the line Zin is affected by the terminating element ZL as:

Z_{in}= Z0

Z_{L}+ Z0tanh jβ` + α`

Z0+ ZLtanh jβ` + α`

. (1.20)

This relationship is known as the transformation of impedances. We can use it to show the equivalence in behaviour between short-circuited transmission lines and series resonating circuits, and between open-circuited transmission lines and parallel resonating circuits.

2_{On nondispersive lines, signal speed is independent of frequency.}

3_{Common dielectric materials used as substrates in superconducting quantum computing include silicon,}

with a low temperature loss tangent of less than 12 × 10−6 and sapphire with a loss tangent of less than 10 × 10−6 [12].

A short circuited transmission line has ZL= 0 and thus the transformation of impedances

reduces to Zin= Z0tanh (jβ` + α`). Applying tanh identities,

Zin =

tanh α` + j tan β`

1 + j tanh β` tan α` (1.21)

Shorted transmission line resonators are also called λ/2 resonators due to the fact that they support a resonance at the frequency for which the length of the line is ` = λ0/2,

where λ0 = c0/f0 = 2πc0/ω0 is the resonant wavelength of the line.4 We can confirm this

behaviour by substituting ` = λ0/2 into (1.21) above. Assuming small deviations around

ω05 and low loss,6 we eventually obtain

Zin =

1

2r` + jl`∆ω (1.22)

which is identical to (1.9) for a series resonant circuit.

We can determine a function for the quality factor in terms of transmission line pa-rameters by substituting (1.19) and (1.18) into (1.7), noting that L = l` and R = r` . Then:

Qs = β

2α. (1.23)

Here, the quality factor is the ratio between propagation and attenuation. If we can determine the values of α and β for a transmission line, regardless of geometry, we can determine the internal quality factor.

A similar derivation can be performed for an open circuited transmission line, where 1/ZL = 0. We call these lines λ/4 resonators, and when substituting ` = λ0/4, the

transformation of impedances reduces to Zin =

1

2r` + jl`∆ω (1.24)

which is identical to the case of the short circuited λ/2 line.

4_{c}

0 is the speed of light in the line material.
5 _{If we assume small deviations ∆ω around ω}

0 so that ω = ∆ω + ω0, we can say β` = `ω/c0 =

(`/c0)(ω0+ ∆ω) = π(1 + ∆ω/ω0).

6 _{For small losses, we can assume α` 1, so tanh (α`) ≈ α`. For small losses and small deviations}

### 1.1.3

### Modes

In this section, we build an understanding of multimode systems so we can apply it to the CPW resonator. This section is based on the treatment of modes in Collin [9] and Mariantoni [10].

A resonant line sustains a set of sinusoidal standing waves whose node and antinode
locations7 _{are determined by its terminating elements. These sets of standing waves, or}

modes, are comprised of frequencies

fm−1 = mf0, (1.25)

m = 1, 2, 3, ... for λ/2 lines, and

fm = (2m + 1)f0, (1.26)

m = 0, 1, 2, ...

for λ/4 lines, where f0 = c0/λ0 is the fundamental resonant frequency.

Lumped element resonators sustain only a single mode, whereas distributed element resonators sustain sets of modes.

Transmission lines often support modes that have some missing electric or magnetic field components. Transverse electromagnetic (TEM) modes have Ez = Hz = 0, whereas

transverse electric and transverse magnetic modes have simply Ez = 0 and Hz = 0,

respec-tively. These vanishing components simplify the associated Maxwell’s equations and allow us to solve for electric and magnetic field propagation equations [9]. CPWs can be said to sustain quasi-TEM modes, which can be approximated as TEM modes in order to garner greater understanding of CPW behaviour [11].

### 1.1.4

### Resonator quantization

Thus far, we have only considered classical resonators as models for the superconducting microwave resonator. In order to fully understand these devices, we must describe them

7_{A node is a position where the standing wave is stationary, i.e., sin βz = 0. Conversely, an antinode}

is a position where the wave amplitude is at its maximum. Nodes and antinodes are useful tools in superconducting quantum computing, as they can be used to minimize or maximize the coupling between neighbouring devices.

using quantum concepts such as the quantum mechanical Hamiltonian. This section is based on the treatment of resonator quantization in Mariantoni [10].

The Hamiltonian for a lossless resonator, modeled as a lumped LC circuit, is
ˆ
H = 1
2C ˆV
2_{+} 1
2L ˆI
2 _{(1.27)}
= Qˆ
2
2C +
ˆ
Φ2
2L

with charge on the capacitor ˆQ = C ˆV and inductor flux ˆΦ = L ˆI. In analogy to the momentum and position operators, the two observables follow the commutation relation

[ ˆQ, ˆ_{Φ] = j~.} (1.28)

If we define lowering and raising operators ˆa and ˆa† in terms of ˆQ and ˆΦ as in

ˆ a = √ 1 2C~ω( ˆQ + jCω ˆΦ) (1.29) and ˆ a† = √ 1 2C~ω( ˆQ − jCω ˆΦ) (1.30)

with commutation relation [ˆa, ˆa†] = 1, we can rewrite (1.27) as

ˆ

HLC = ~ω(ˆa†a +ˆ

1

2) (1.31)

which is the Hamiltonian for a one-dimensional quantum harmonic oscillator (QHO). Thus we have shown the transformation from LC resonant circuit to QHO.

The resonator eigenvalue n and eigenket |ni can be determined using ˆ

N |ni = ˆa†ˆa |ni = n |ni (1.32) since lowering operator

ˆ

a |ni =√n |n − 1i (1.33)

and raising operator

ˆ

a†=√n + 1 |n + 1i . (1.34)

The energy levels can be found by

n = 0, 1, 2, ...

Unlike a classical resonator, the QHO has nonzero energy E0 = ~ω/2 in its ground state.

Each mode behaves as a QHO. For a λ/2 resonator,
ˆ
H_{λ/2} =
∞
X
m=1
~ωm(ˆa†mˆam+
1
2) (1.36)
m = 1, 2, 3, ...

where ωm = mω0 is the frequency of mode m, and ˆa†m and ˆam are the raising and lowering

operators for mode m.

### 1.1.5

### The coplanar waveguide

In this section, we will explore analytical descriptions of the characteristic impedance Z0

and effective permittivity ef f of the CPW. These parameters are geometry-dependent and

must be accounted for during device design. It is often important to design transmission lines to be 50 Ω matched, i.e. Z0 = 50 Ω, as external wiring usually has the same impedance

and reflections can result from impedance mismatches, leading to loss. Effective permit-tivity affects the internal quality factor of the device, and should be taken into account (see Chapter 3 for more details). This section is based on the sources of Simons [11] and Mohebbi [13].

The standard CPW

The standard coplanar waveguide (CPW) consists of a metallic thin film separated into centre conductor and ground planes on either side, all of which sits on top of a dielectric substrate (Fig. 1.4 (a)). As stated in Sec. 1.1.3, CPWs sustain quasi-TEM modes. These devices are simple to fabricate and have low radiation loss compared to other waveg-uides [11].

Using conformal mapping8, we can determine formulae for the characteristic impedance Z0and effective dielectric constant ef f for a standard CPW. For a CPW [Fig.1.4(a)] made

8 _{Conformal mapping is the mapping of one set of variables to another while preserving local angles.}

The CPW boundaries for the Laplace equation can be mapped to a set of boundaries where a solution is more easily found. Refer to Appendix III: Conformal Mapping Techniques in Simons [11] for more information.

of an infinitely thin superconductor with gap width w and conductor width s on a dielectric of some finite thickness h with dielectric constant rd, [11]

ef f = 1 +
(rd− 1)
2
K(k1)
K(k0_{1})
K(k_{0}0)
K(k0)
(1.37)
and
Z0 =
30π
√
ef f
K(k0_{0})
K(k0)
(1.38)
where K(k_{n}) are complete elliptic integrals of the second kind9 _{with inputs}

k0 =

s

s + 2w, (1.39)

which is the CPW aspect ratio, and

k_{0}0 =
q
1 − k2
0 (1.40)
k1 =
sinhπs
4h
sinh π(s + 2w)
4h
(1.41)
k0_{1} =
q
1 − k2
1. (1.42)

Assuming a substrate of infinite thickness, (1.37) and (1.38) become
_{ef f} = 1 + rd
2 (1.43)
Z0 =
30π
p(_{ef f} + 1)/2
K(k0_{0})
K(k0)
. (1.44)

When h < 2w, there is a 10% - 15% error when using the assumption of infinite thickness. For the case of standard superconducting quantum circuits such as the ones used in this thesis, h ' 500um and w ' 10um, so we are free to use either set of equations.

9 _{Complete elliptic integrals of the second kind can be expressed as an integral or as a power series,}

K(k) = π_{2}P∞

We can also use more accurate expressions which takes into account the superconduc-tivity, and thus the surface impedance, of a CPW with superconducting thin film [13]. These expressions are

q
t
ref(f ) =
q
t
ref(0) +
√
rd−
q
t_{ref}(0)
1 + g(f /fT E)−1.8
(1.45)
and
Z0 =
30π
q
t_{ref}
K(k0_{0})
K(k0)
(1.46)
where
t_{ref}(0) = ref(0) −
0.7(ref(0) − 1)(t/w)
K(k0)
K0_{(k}_{0}_{)}+ 0.7(t/w)
(1.47)
ref(0) = 1 + q(rd− 1) (1.48)
q = 1
2
K(k1)K(k00)
K(k0_{1})K(k0)
. (1.49)
and
g = eu ln (s/w)+v (1.50)
fT E =
c0
4h√rd− 1
(1.51)
u = 0.54 − 0.64p − 0.015p2 (1.52)
v = 0.43 − 0.86p + 0.54p2 (1.53)
p = ln s
h (1.54)

where c0 is the speed of light, f is the frequency, and t is the superconducting film thickness.

The capped CPW

Adding a cap to a CPW can suppress loss by shielding it from the environment. We can model the capped coplanar waveguide (described in Chapter 3) as a CPW with a second dielectric above the CPW (air) and a third ground plane above that (Fig. 1.4 (b)). The general form of this device is called a grounded CPW (GCPW). Simons [11] refers to this

(a) (b) s w s w h t r d s w h2 t h1 r d

Figure 1.4: Diagram of standard CPW (a) with top and orthographic views and GCPW (b) with orthographic view. The substrate (yellow) is of thickness h (h1) and dielectric

constant rd. The metal (grey) has thickness t and is patterned with gaps of width w and

device as a “conventional coplanar waveguide on a finite thickness dielectric substrate and with a top metal cover”. Dielectric permittivity and characteristic impedance are given as

ef f = 1 + q3(rd− 1) (1.55)
and
Z0 =
60π
√
_{ef f}
1
K(k0)
K(k_{0}0) +
K(k4)
K(k_{4}0)
(1.56)
where
q3 =
K(k1)
K_{k}0
1
K(k0)
K(k_{0}0)+
K(k4)
K(k0_{4})
(1.57)
k4 =
tanh (πs/4h2)
tanh (π(s + 2w)
4h2
)
(1.58)
k_{4}0 =
q
1 − k2
4 (1.59)

where h2 is the height of the cap.

### 1.2

### The qubit

The superconducting qubit is a circuit that consists of the combination of a resonator and a nonlinear inductive element, the Josephson junction. Adding a nonlinear element to a resonator changes its energy levels so that they are non-uniformly distributed, thereby allowing energy gaps to be addressed individually.

The Josephson junction, or Josephson tunnel junction, is the combination of two su-perconducting leads weakly connected by a constriction, a normal metal, or a thin in-sulator [14]. In superconducting quantum computing, the connection is most commonly formed from an insulator such as aluminium oxide.

The Josephson junction has a critical current I_{c0} which is the maximum dc current that
can be supported by the junction. Within those bounds, the supercurrent Is can be found

by

where ∆ϕ is the superconducting wave function’s phase difference across the junction. Above the critical current,

d dt∆ϕ =

2e ~

V (1.61)

where V is the voltage drop across the junction.

We can use these relationships to show that the Hamiltonian for a qubit is ˆ H = Qˆ 2 2C + ˆ Φ2 2L − EJcos Φ (1.62)

where the first two terms are due to the resonator (Sec. 1.1.4) and the last term is due to the Josephson junction.

### 1.3

### Two level system loss

Superconducting quantum devices inevitably contain some amount of amorphous dielectric
material. Common materials include native oxide (such as silicon, aluminium or indium
surface oxide) and grown oxide (such as aluminium oxide grown to form a Josephson
junc-tion). At temperatures T < 1K, [15] these materials cause loss which can be modeled as
two level system (TLS) loss. TLSs absorb photons and phonons from a superconducting
device via electric field coupling and then spontaneously re-emit them. At high
tempera-tures or high powers, these systems become saturated due to excess energy in the system,
and therefore do not cause much loss10_{. However, at low powers, the interaction is quite }

sig-nificant. TLS loss is largely the limiting form of loss in superconducting quantum circuits at low temperature, [16] and by understanding TLS loss we can improve the performance of these circuits. TLS loss varies depending on the materials present, so modeling TLS loss is a method of characterizing materials in terms of their superconducting microwave performance.

We can determine the TLS component of loss for a superconducting CPW resonator by comparing its resonant frequency’s temperature dependence or its loss tangent’s power dependence to the same dependences for the TLS model. Below, the TLS model is looked at in greater depth, and the two dependences are derived, following the primary sources of Anderson [17] and Phillips [15,18] and the secondary sources of Gao [19] and Pappas [20]. Amorphous materials have been theorized to contain atoms or atomic clusters that tun-nel between pairs of locations, acting as a particle in an asymmetric double well potential

V1

V2

H1 H2

∆0

∆

Figure 1.5: Potential energy diagram for a double well potential, showing each potential separately (left) and as a single merged potential (right). The wells have Hamiltonians H1 and H2, minimum potentials V1 and V2, asymmetry energy ∆, and tunneling matrix

element ∆0.

(Fig.1.5). Under applied electric field ~E = E ˆe, the double well potential has electric dipole moment ~D = d ˆd which characterizes its ability to couple to external photons. TLSs also have an elastic dipole moment which couples to the strain field of the system and allows phonon coupling.

Each of these double well potentials has a distinct asymmetry energy ∆ (energy differ-ence between the two potential wells) and tunneling matrix element ∆0 (change in energy

due to tunneling). These values are produced via the random structure of the amorphous material and are therefore part of a broad distribution. Commonly, ∆ is assumed to have a uniform distribution and ∆0 a logarithmic distribution. An in-depth discussion on the

distribution of these variables can be found in Phillips [15].

### 1.3.1

### The two level system Hamiltonian

For two single well potentials with Hamiltonians H1 and H2 and minimum potentials V1

and V2, the Hamiltonian of the double well potential is H = H1+ (V − V1) = H2+ (V − V2)

or, in a simplified matrix form,

H = 1
2
−∆ ∆_{0}
∆0 ∆
(1.63)
for the local basis consisting of ground states of the single well problems, φ1 and φ2.

Defining θ = 1_{2}arctan∆0

∆, eigenstates are

ψ2 = φ1sin θ − φ2cos θ (1.65)

with eigenenergies ±E/2 where E =p∆2_{+ ∆}2

0. Diagonalizing the Hamiltonian with basis

states ψ1 and ψ2, we obtain the usual two level system Hamiltonian,

H0 = 1 2Eσz = 1 2E 1 0 0 −1 (1.66) where σz is the Pauli z matrix. The interaction Hamiltonian with both an electric and

strain field is Hint= ( ∆ Eσz+ ∆0 E σx) ~d0· ~E (1.67) where ~d0 is the maximum dipole moment and ~E is the electric field. For a more detailed

treatment of the two level system Hamiltonian, see Gao [19].

### 1.3.2

### Dielectric contribution of TLSs

The TLS model’s power v.s. loss and resonant frequency v.s. temperature relationships can be found through the TLS dielectric contribution term

T LS(ω) = Z Z Z [ˆe · ~~χres(ω) · ˆe] P ∆0 d∆d∆0d ˆd (1.68)

where P is the density of states and ~χ is the magnetic susceptibility. With a change of~ variables and by integrating, we can modify this into

T LS(ω) = P d2 3~ Z Emax 0 χres(ω)dω (1.69)

where χres(ω) = χAresχBresχCres, a product of three terms. The first term

χA_{res}= tanh E

2kT (1.70)

takes into account the difference in probability between the ground and excited states. The term

χB_{res}= 1
ωE − ω + i/T2

is the TLS single-pole response under the rotating wave approximation (RWA), where T2

is the phase decoherence lifetime. For energy relaxation lifetime T1 and Rabi frequency

Ω = 2 ~D˙( ~_{E/~), the third term is}

χC_{res}= 1 + (ωE − ω)
2_{T}2
2
1 + Ω2_{T}
1T2+ (ωE − ω)2T22
. (1.72)

This term takes into account TLS saturation. When fields are weak, which is the case at
low powers used in superconducting quantum computing, Ω2_{T}

1T2 << 1, and χCres∼ 1.

Considering only the imaginary component of T LS= 0− i00, we eventually arrive at

tan δ = F tan δ0tanh ~ω 0

2kBT

. (1.73)

where kB is the Boltzmann constant, F is the filling factor of the TLS material, and

tan δ0 is the component of the loss tangent due to TLSs at a temperature of absolute zero.

Considering only the real component, we see
f0(T ) = f0,i
1 + p
ReΨ
~ω0
2πik_{B}T +
1
2
− ln ~ω0
k_{B}T
. (1.74)

where f0,i is the resonant frequency of the resonator at absolute zero, Ψ is the complex

Digamma function, and p = F tan δ0/π.

These two relations can be fitted to determine tan δ0 and f0,i in measured

## Chapter 2

## Moving towards extensibility and

## scalability

The components necessary for a quantum computer are outlined in the DiVincenzo crite-ria, [21] the first being

“A scalable physical system with well characterised qubits.”

In this thesis, scalability is used loosely to refer to the ability to increase the number of elements, connections, and computing power of a system. Currently, many challenges lie in the path of further scaling of superconducting quantum circuits. Box modes due to sample holders, as well as chip modes, limit chip size, and crosstalk and slotline modes become are exacerbated when chips are densely covered with devices. Further, we do not fully understand the causes of loss in these devices, making it difficult to optimize device performance.

In this chapter, we begin by introducing the issue of unwanted modes and coupling in extensible superconducting quantum circuits. Next, we examine multilayer superconduct-ing quantum architectures which could act as a solution to unwanted modes and couplsuperconduct-ing and allow us to further scale the superconducting quantum circuit. Finally, we introduce the study of materials used in superconducting quantum circuits, especially indium, an essential component to the multilayer architecture.

### 2.1

### Understanding and suppressing unwanted modes

### and coupling

Resonances within the 4-8 GHz working frequency region that were not purposefully
de-signed can be referred to as unwanted modes.1 _{Unwanted modes can interfere with }

compu-tations and measurements of a superconducting circuit, and can lead to decoherence and radiation loss [22, 23]. These modes originate from many different sources, including the sample holder geometry (box modes) and resonator meandering or uneven ground planes (slotline modes). Interactions between neighbouring devices (crosstalk) can have similar consequences. Suppression of the above modes has been attempted in various ways, both successfully and unsuccessfully. This section will elaborate on the nature and cause of commonly seen unwanted modes and coupling, and outline past and current attempts to suppress them in the field of superconducting quantum computing.

### 2.1.1

### Slotline modes

Parasitic slotline modes, or simply slotline modes, are a type of odd mode that occur when ground planes are not electrically connected or are uneven in width, leading to a voltage differential across the coplanar waveguide.

Ground planes become disconnected from one another when the design of the chip is such that sections of ground are enclosed by transmission lines or other components. Disconnected ground planes become inevitable in a planar circuit growing in complexity. Uneven ground planes can be caused by a bend in the transmission line or an asymmetric circuit design where a device lays close to one side of a transmission line but not the other. Some type of connection is necessary in order to eliminate loss due to slotline modes [24]. Two common crossover solutions are used: wire bonds and air bridges.

Wire bonds

It is common practice to ground a chip’s ground planes by wire bonding them to a metal base below the chip (Fig.2.1). However, due to the poor shielding of wire bonds, crosstalk between neighbouring wire bonds cause this type of ground connection scheme to fail for larger chip sizes [25].

1_{Modes that fall outside of the 4-8 GHz range will not couple to on-chip devices and thus will not affect}

Wire bonds can also be used within a chip to connect ground planes across transmission lines and resonators. The small physical size of wire bonds leads to local grounding only, so a dense, uniform covering of wire bonds is necessary for good grounding.[26] Wire bonds also add inductance to the line [25, 26].

Finally, wire bonding can be performed onto pads at the edges of each chip in order to connect to external electronics for qubit control and measurement. However, this method does not allow connections to qubits located within a qubit array or complex circuit, as connections can only be made near the edges [27].

Air bridges

Air bridges (Fig. 2.1) are metallized freestanding structures which connect the ground on one side of a transmission line or resonator to the other [24, 26, 28, 29]. They are fabricated using standard photolithography methods and are generally seen as a more convenient alternative to wire bonding. While wire bonds add inductance to the line, air bridges add shunt capacitance [26].

A density of 10 air bridges per nm has been shown to fully attenuate slotline modes.[24] Chen et al. [24] notes an air bridge success rate of > 99.9%. Some studies suggest that air bridges are fragile, and can fail as a result of an ultrasonic bath [24, 29]. Extrapolating from loss experiments in Chen et al., [24] a resonator fully covered by air bridges would have an internal quality factor limited to 120,000 at low power [24]. The source of this loss is unclear but it is considered to be TLS loss due to its power dependence.

### 2.1.2

### Crosstalk

Crosstalk is the exchange of signals between neighbouring lines or devices. Unintended crosstalk can occur when devices are close together. Sufficient separation of devices spa-tially or in frequency can mitigate crosstalk. However, as circuits become larger and denser, sufficient separation becomes more difficult to achieve.

One possible solution to crosstalk is to add some kind of shielding element between devices to block the signal, as proposed by Abraham et al. [30–32] In this scheme, a metallized cap chip containing a cavity is placed over the device chip, grounding the device’s ground planes through a large capacitance between the two metallized layers.

Martinis and Megrant [33] measured a nine qubit circuit with conductor width 3µm, gap 1.5µm, and line separation 200 µm, and measured microwave crosstalk in the range of

Figure 2.1: Physical implementations of two common solutions to parasitic slotline modes. Left: Photograph of a chip in a sample mount with wire bonds connecting to ground planes around the edges of the chip, and spanning an on-chip resonator, reproduced from [25]. Right: Scanning electron microscope image of an air bridge spanning a coplanar transmission line, reproduced from [26].

Crosstalk is also an issue between neighbouring wire bonds, as wire bonds are poorly shielded from the environment. This leads to significant loss in superconducting quantum circuits. Wire bonds are observed to have isolation2 around 20 dB [27].

A possible solution to wire bond crosstalk is their replacement with another wiring scheme such as three-dimensional (3D) wiring [27]. By using 3D wiring and associated packaging (Fig. 2.2), crosstalk can be lowered to -45 dB in the dc to 10 GHz range. This set-up consists of a set of coaxial pogo pins embedded into the lid of the sample box. When the lid is put in place, the pins make contact with pads on the chip to connect to control and measurement electronics. The pin has a centre conductor which hits a pad connecting to an on-chip transmission line, while the outer ground of the pin makes contact with the on-chip ground plane. The package lid holds a washer spring at each corner which, when base and lid are assembled, make contact with the washer surrounding the chip and form a ground.

2_{Isolation is the opposite of crosstalk; it is the magnitude of the signal that does not leak to neighbouring}

Figure 2.2: Image of a microwave package containing a set of six three-dimensional wires, reproduced from [27]. A chip is shown in the base under the washer, and four washer springs are located in the lid above each washer pillar. Six pogo pins are shown embedded in the package lid.

Figure 2.3: Cross-sectional diagram of a shielded coplanar transmission line designed to suppress unwanted modes and crosstalk, reproduced from [30]. 101: Cap chip. 108: Cap metallization. 105: Empty cavity. 106: Chip substrate. 102 and 104: Metallized CPW ground planes. 103: Metallized CPW centre conductor.

### 2.1.3

### Box modes

Box modes are modes sustained within the free space in the sample box where the super-conducting quantum circuit chip is held for cooldown and measurement (an example of a box used in cooldowns in this work is shown in Fig.2.2). The frequencies of these modes depend on the geometry of the box. The fundamental frequency of the box is inversely related to its proportions: as the sample box grows in size, the fundamental frequency, and thus all of the modes associated with the box, become lower. If the box geometry is large enough, some box modes will fall within the superconducting circuit working range of 4-8 GHz and interfere with on-chip devices.

We can intentionally raise box mode frequencies by modifying the geometry or boundary conditions of the cavity. For example, adding an evacuated space below the chip (such as in Fig.2.4) raises the box modes [27]. The addition of coaxial pogo pins has a similar effect by changing the electromagnetic boundary conditions [34]. Fig.2.5 shows an architecture of 89 pogo pins of diameter 500µm which increase the fundamental mode of the 72 mm × 72 mm × 3 mm sample box above 12 GHz.

Figure 2.4: Cross-sectional diagram of a sample box (grey) and chip (green) with under-chip cavity for increasing the fundamental box mode frequency, and support pillar beneath the chip for stability. Vacancy line on the left is for pumping the chip cavity to vacuum. For scale, chip has a width of 15 mm. Photography of similar sample box can be found in Fig.2.2. Image reproduced from [27].

### 2.1.4

### Identifying unwanted coupling

Cavity modes such as box or chip modes (chip modes being modes sustained by the chip substrate) can be distinguished from other modes as they are visible in the spectrum both at room temperature when no superconductivity occurs and at low temperature, as they do not depend on superconductivity in order to exist. Box modes will be suppressed once the box cavity is interrupted (say, by being filled with material), but chip modes will not be affected by this as they are sustained by the chip and not the cavity. Thus, we can distinguish between these two types of modes by adding a filler within the empty space of the box [25].

Slotline modes and resonator frequencies can be distinguished experimentally by fab-ricating one chip with normal resonators and one where the resonators lack a centre con-ductor. Modes that occur in both samples are slotline modes, while modes that occur only in the first sample are designed resonances due to the coupled resonators [25].

### 2.2

### Multilayer quantum devices

The expansion of superconducting quantum circuits into the third dimension can allow us to realize larger and denser qubit arrays, as well as facilitate more complex coupling schemes and architectures. As a solution to the scalability issues plaguing the

supercon-Figure 2.5: Simulation of the electric field magnitude || ~E|| of the first box mode in a 72 mm × 72 mm × 3 mm sample box containing 89 coaxial pogo pins. Due to the pogo pins, the first box mode is raised to a frequency of 12.295 GHz. Image reproduced from [34].

quantum circuit (MMIQC), an architecture which takes advantage of the third dimension to lower the footprint of the quantum circuit.

The MMIQC architecture consists of stacked arrays of on-chip circuits enclosed within individual 3D cavities and connected by shielded superconducting transmission lines within the same layer and vias between layers (Fig.2.6). First steps of this architecture have been demonstrated, with a micromachined resonant cavity [36] and a 3D transmon qubit inside a cavity [37].

Variations on this architecture have also been pursued. Rosenberg et al. [38] proposes a simpler near-term architecture in the same vein consisting of a base chip supporting qubits, and a cap chip supporting wiring and Josephson junctions for signal amplification. The two chips are connected through an interposer containing through-silicon vias and planar wiring using indium bump bonding. Initial testing of this architecture has been performed with transmon qubits on a separate chip as their control and readout lines.

Multilayer quantum devices have the advantage of being able to efficiently implement shielding of unwanted modes and crosstalk as shown in Fig. 2.3 and Fig. 2.6. This type of shielding can be performed by embedding a metallized cavity into the underside of a chip and placing it over the devices of interest. Multilayer quantum devices also have the benefit of being able to segregate devices to separate chips depending on their fabrication and performance requirements. For example, resonators, transmission lines, and other ancillary devices can be removed from the high performance qubit chip [38] in order to decrease the amount of processing and thus the likelihood of contamination of the qubits. This allows greater fabrication precision and the possibility of qubits with higher coherence times.

### 2.2.1

### Indium in multilayer quantum circuits

With the rising interest in multilayer quantum circuits, indium has become a material of interest both for die bonding and for signal propagation purposes. Indium is a low temperature superconductor with a critical temperature Tc = 3.4 K. It is a commonly

deposited thin film with high purity targets readily available for purchase. Due to its physical malleability and low melting point (157◦C compared to aluminium’s 660◦C), indium is an ideal solder.

Indium bump bonds are a common bonding tool in the semiconductor industry that has recently been embraced by the field of superconducting quantum computing. This method is used to bond pairs of silicon wafers and electrically connect their on-chip circuits [38–

Figure 2.6: A diagram of the proposed microwave multilayer integrated quantum circuit consisting of metallized micromachined silicon cavities functioning as 3D resonators and shields, through-silicon vias for interconnection of layers, on-chip transmission lines and resonators, and qubits residing on a membrane (green), all connected by thin film bonding. Image reproduced from [35].

40]. Indium bump bonds are fabricated by patterning an indium film several microns thick. These bumps can then be used to cold bond two dies together under pressure.

Interdiffusion can occur between aluminium and indium films [41]. This phenomenon reduces the performance of devices, although the loss mechanism is unclear. Under bump metallization (UBM) is used in indium bump bonding in order to suppress diffusion be-tween these metals [38]. Common UBM materials include titanium nitride, a non-oxidizing, high-Q superconductor, as well as stacks such as titanium/platinum/gold, [38] molybde-num/titanium, and titanium/palladium [39].

Rosenberg et al. [38] demonstrated 2,704 bump bonds in series with a resistance of 240 nΩ per bump at superconducting temperatures (< 1 K). In contrast, Foxen et al. [42] measured a resistance of < 3 nΩ per bump for a chain of 1,620 indium bumps, demonstrat-ing what is essentially superconductdemonstrat-ing indium bump bonddemonstrat-ing. These bumps were bonded between a lower silicon substrate with aluminium circuits and titanium nitride UBM, and a silicon cap with indium wiring. O’Brien et al. [39] demonstrated a device capping method using indium bump bonds.

## Chapter 3

## Indium thin film thermocompression

## bonding for multilayer

## superconducting quantum circuits

The majority of this chapter was published on 2017 September 18 as [1] :McRae, C.R.H., B´ejanin, J.H., Pagel, Z., Abdallah, A.O., McConkey, T.G., Earnest, C.T., Rinehart, J.R., Mariantoni, M. Thermocompression Bonding Technology for Multi-layer Superconducting Quantum Circuits. Appl. Phys. Lett. 111, 123501 (2017).

The list of author contributions can be found in the Statement of Contributions within the front matter of this thesis.

As mentioned in Chapter2, a large array of low error rate quantum devices is necessary in order to implement an extensible or scalable quantum computing architecture. Stack-ing microchips of various functionalities into multilayer superconductStack-ing quantum ciruits (Sec.2.2) is a promising, up-and-coming method of scaling quantum processors.

The following section consists of the experimental demonstration of a
thermocompres-sion bonding technology that utilizes indium films as a welding agent to attach pairs
of lithographically patterned chips. We perform chip-to-chip indium bonding in vacuum
at 190◦C with indium film thicknesses of 150 nm. We characterize the dc and microwave
performance of bonded devices at room and cryogenic temperatures. At 10 mK, we find
a dc bond resistance of 49.2µΩ cm2_{. Additionally, we show minimal microwave reflections}

and good transmission up to 6.8 GHz in a tunnel-capped, bonded device as compared to a similar uncapped device. As a proof of concept, we fabricate and measure a set of

tunnel-capped superconducting resonators, demonstrating that our bonding technology can be applied to superconducting quantum computing.

### 3.1

### Introduction

The field of quantum computing [5] is experiencing major growth thanks to the devel-opment of architectures with ten or more quantum bits (qubits) [43, 44]. The biggest challenge in the realization of a universal quantum computer is the implementation of ex-tensible architectures where qubit operations can be performed with low error rates [45]. Among many promising qubit architectures, [46–49] those based on superconducting quan-tum circuits [50] are rapidly reaching a level of maturity sufficient to demonstrate the su-periority in peformance of a digital quantum computer over the state-of-the-art classical supercomputer [8]. Elements of quantum error correcting codes [6, 7] have already been demonstrated in a variety of experiments using superconducting qubits [44, 51, 52] and a quantum memory has been realized with quantum states of microwave fields [53].

In order to build an extensible quantum computer, however, many technological ad-vances must first be demonstrated. Among these, three-dimensional integration and pack-aging of superconducting quantum circuits is emerging as a critical area of study for the realization of larger and denser qubit architectures. This approach allows the departure from the two-dimensional confinement of a single microchip to a richer configuration where multiple chips are overlaid. Three-dimensional integration, thus, provides a flexible plat-form for more advanced classical manipulation of qubits and qubit protection from the environment. In this framework, an architecture based on multilayer microwave integrated quantum circuits has been proposed [54] and some of its basic elements realized, showing that high-quality micromachined cavities [35] can be used to implement three-dimensional superconducting qubits [37]. Leveraging the extensive body of work developed in the con-text of classical integrated circuits, flip chip technology has been adopted to bond pairs of microchips containing superconducting circuits [38, 40, 55]. Furthermore, high frequency through-silicon vias [56] and a quantum socket based on three-dimensional wires [27] have been developed to attain dense connectivity on a two-dimensional array of qubits.

In this work, we demonstrate the experimental implementation of a two-layer integrated superconducting circuit where two microchips are attached by means of thermocompression bonding in vacuum. The structures on the surface of the bottom chip (or base chip) and on the underside of the top chip (or cap chip) are fabricated using standard photolithography techniques. Instead of a discrete set of indium bump bonds, a continuous thin film of

(a) (b) (c) (d) T S W H 3 mm 700 µm

Figure 3.1: Capped devices formed using thermocompression bonding in vacuum. (a) Cutaway diagram of a capped device, exposing aluminium (dark green) and indium (light blue) films. The CPW transmission line features a center conductor of width S = 12µm and gaps of width W = 6µm. The tunnel height is H = 20 µm, with width T = 175 µm (see inset). Through holes in the cap allow electrical connection to the base chip by means of three-dimensional wires [27]. (b) Macrophotograph of a bonded sample. Inset: Microimage of a through hole showing a conductor trace aligned with a tunnel. (c) Cross section of a bonded sample showing six tunnels (dark gray rectangles). (d) Detail of a tunnel in (c).